 
data_RWJMN
 
_audit_creation_method            SHELXL-2013
_chemical_name_systematic
;
 ?
;
#===============================================================================
# 1. SUBMISSION DETAILS
_publ_contact_author_name      'Prof. Dr. Jin-Xiao Mi'
_publ_contact_author_address
;
Department of Materials Science and Engineering
College of Materials,
Xiamen University,
Xiamen 361005, Fujian Province
People's Republic of China
;
_publ_contact_author_phone     '0086-13696905136'
_publ_contact_author_fax       '0086-592-2183937'
_publ_contact_author_email     'jxmi@xmu.edu.cn'
_publ_requested_journal         ?
_publ_requested_category        ?
_publ_requested_coeditor_name   ?
_publ_contact_letter
;
Jan 10, 2015

Please consider this CIF submission for deposit ICSD. 
All authors have seen and approved this submission. 
The authors acknowledge the conditions of publication.

The CIF has passed the enCIFer(V1.1) checking.

Jin-Xiao Mi
;
#===============================================================================


_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'F12 H18.78 K3.74 Mn7 Na8 O40.26 P8' 
_chemical_formula_weight          1853.58

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na'  'Na'   0.0362   0.0249
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'K'  'K'   0.2009   0.2494
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mn'  'Mn'   0.3368   0.7283
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P'  'P'   0.1023   0.0942
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'F'  'F'   0.0171   0.0103
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       cubic
_space_group_IT_number            202
_space_group_name_H-M_alt         'F m -3'
_space_group_name_Hall            '-F 2 2 3'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 '-x, -y, z'
 'x, -y, -z'
 '-x, y, -z'
 'z, x, y'
 '-z, -x, y'
 'z, -x, -y'
 '-z, x, -y'
 'y, z, x'
 'y, -z, -x'
 '-y, z, -x'
 '-y, -z, x'
 'x, y+1/2, z+1/2'
 '-x, -y+1/2, z+1/2'
 'x, -y+1/2, -z+1/2'
 '-x, y+1/2, -z+1/2'
 'z, x+1/2, y+1/2'
 '-z, -x+1/2, y+1/2'
 'z, -x+1/2, -y+1/2'
 '-z, x+1/2, -y+1/2'
 'y, z+1/2, x+1/2'
 'y, -z+1/2, -x+1/2'
 '-y, z+1/2, -x+1/2'
 '-y, -z+1/2, x+1/2'
 'x+1/2, y, z+1/2'
 '-x+1/2, -y, z+1/2'
 'x+1/2, -y, -z+1/2'
 '-x+1/2, y, -z+1/2'
 'z+1/2, x, y+1/2'
 '-z+1/2, -x, y+1/2'
 'z+1/2, -x, -y+1/2'
 '-z+1/2, x, -y+1/2'
 'y+1/2, z, x+1/2'
 'y+1/2, -z, -x+1/2'
 '-y+1/2, z, -x+1/2'
 '-y+1/2, -z, x+1/2'
 'x+1/2, y+1/2, z'
 '-x+1/2, -y+1/2, z'
 'x+1/2, -y+1/2, -z'
 '-x+1/2, y+1/2, -z'
 'z+1/2, x+1/2, y'
 '-z+1/2, -x+1/2, y'
 'z+1/2, -x+1/2, -y'
 '-z+1/2, x+1/2, -y'
 'y+1/2, z+1/2, x'
 'y+1/2, -z+1/2, -x'
 '-y+1/2, z+1/2, -x'
 '-y+1/2, -z+1/2, x'
 '-x, -y, -z'
 'x, y, -z'
 '-x, y, z'
 'x, -y, z'
 '-z, -x, -y'
 'z, x, -y'
 '-z, x, y'
 'z, -x, y'
 '-y, -z, -x'
 '-y, z, x'
 'y, -z, x'
 'y, z, -x'
 '-x, -y+1/2, -z+1/2'
 'x, y+1/2, -z+1/2'
 '-x, y+1/2, z+1/2'
 'x, -y+1/2, z+1/2'
 '-z, -x+1/2, -y+1/2'
 'z, x+1/2, -y+1/2'
 '-z, x+1/2, y+1/2'
 'z, -x+1/2, y+1/2'
 '-y, -z+1/2, -x+1/2'
 '-y, z+1/2, x+1/2'
 'y, -z+1/2, x+1/2'
 'y, z+1/2, -x+1/2'
 '-x+1/2, -y, -z+1/2'
 'x+1/2, y, -z+1/2'
 '-x+1/2, y, z+1/2'
 'x+1/2, -y, z+1/2'
 '-z+1/2, -x, -y+1/2'
 'z+1/2, x, -y+1/2'
 '-z+1/2, x, y+1/2'
 'z+1/2, -x, y+1/2'
 '-y+1/2, -z, -x+1/2'
 '-y+1/2, z, x+1/2'
 'y+1/2, -z, x+1/2'
 'y+1/2, z, -x+1/2'
 '-x+1/2, -y+1/2, -z'
 'x+1/2, y+1/2, -z'
 '-x+1/2, y+1/2, z'
 'x+1/2, -y+1/2, z'
 '-z+1/2, -x+1/2, -y'
 'z+1/2, x+1/2, -y'
 '-z+1/2, x+1/2, y'
 'z+1/2, -x+1/2, y'
 '-y+1/2, -z+1/2, -x'
 '-y+1/2, z+1/2, x'
 'y+1/2, -z+1/2, x'
 'y+1/2, z+1/2, -x'
 
_cell_length_a                    15.968(2)
_cell_length_b                    15.968(2)
_cell_length_c                    15.968(2)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma                 90
_cell_volume                      4071.5(15)
_cell_formula_units_Z             4
_cell_measurement_temperature     173(2)
_cell_measurement_reflns_used     6146 
_cell_measurement_theta_min       2.209 
_cell_measurement_theta_max       27.931 
 
_exptl_crystal_description        'Octahedra' 
_exptl_crystal_colour             'rosy-red' 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_method     ?              
_exptl_crystal_density_diffrn     3.024          
_exptl_crystal_F_000              3612
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?   
_exptl_crystal_size_max           0.270
_exptl_crystal_size_mid           0.270
_exptl_crystal_size_min           0.270
_exptl_absorpt_coefficient_mu     3.067
_shelx_estimated_absorpt_T_min    0.491
_shelx_estimated_absorpt_T_max    0.491
_exptl_absorpt_correction_type    'multi-scan'  
_exptl_absorpt_correction_T_min   0.870 
_exptl_absorpt_correction_T_max   1.000 
_exptl_absorpt_process_details    'SADABS (Bruker, 2001)'   
 
_exptl_special_details
;
 ?
;
 
_diffrn_ambient_temperature       173(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source                    'fine-focus sealed tube'
_diffrn_measurement_device_type   
'Bruker SMART APEX CCD area-detector diffractometer'  
_diffrn_measurement_method        
'1800 images,φ = 0, 90, 180°, χ = 54.74°, Δω=0.3°, Exp time: 15 s.' 
_diffrn_detector_area_resol_mean  ? 
_diffrn_reflns_number             6146
_diffrn_reflns_av_unetI/netI      0.0126
_diffrn_reflns_av_R_equivalents   0.0246
_diffrn_reflns_limit_h_min        -20
_diffrn_reflns_limit_h_max        13
_diffrn_reflns_limit_k_min        -21
_diffrn_reflns_limit_k_max        20
_diffrn_reflns_limit_l_min        -17
_diffrn_reflns_limit_l_max        20
_diffrn_reflns_theta_min          2.209
_diffrn_reflns_theta_max          27.931
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.996
_diffrn_measured_fraction_theta_full  0.997
_diffrn_reflns_Laue_measured_fraction_max    0.996
_diffrn_reflns_Laue_measured_fraction_full   0.997
_diffrn_reflns_point_group_measured_fraction_max   0.996
_diffrn_reflns_point_group_measured_fraction_full  0.997
_reflns_number_total              462
_reflns_number_gt                 394
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection        'SMART (Bruker, 2001)' 
_computing_cell_refinement        'SAINT (Bruker, 2001)'  
_computing_data_reduction         'SAINT (Bruker, 2001)'  
_computing_structure_solution     'SHELXL-2013 (Sheldrick, 2013)' 
_computing_structure_refinement   'SHELXL-2013 (Sheldrick, 2013)'
_computing_molecular_graphics     
'DIAMOND (Brandenburg, 2011) & ATOMS (Dowty, 2004)'   
_computing_publication_material   'SHELXL-2013 (Sheldrick, 2013)'
 
_refine_special_details
;
 ?
;
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
;
 w=1/[σ²(Fo²)+(0.0597P)²+19.4949P]
 where P=(Fo²+2Fc²)/3
;
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_number_reflns          462
_refine_ls_number_parameters      43
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0378
_refine_ls_R_factor_gt            0.0329
_refine_ls_wR_factor_ref          0.1057
_refine_ls_wR_factor_gt           0.1038
_refine_ls_goodness_of_fit_ref    1.184
_refine_ls_restrained_S_all       1.184
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Mn1 Mn 0.5000 0.7500 0.7500 0.0189(3) Uani 1 4 d S T P . .
Mn2 Mn 0.5000 0.5000 0.5000 0.0187(5) Uani 1 24 d S T P . .
P11 P 0.35325(8) 0.64675(8) 0.85325(8) 0.0256(5) Uani 0.851(4) 3 d S T P . .
P12 P 0.3275(5) 0.6725(5) 0.8275(5) 0.0256(5) Uani 0.149(4) 3 d S T P . .
Na1 Na 0.37868(8) 0.62132(8) 0.62132(8) 0.0311(6) Uani 1 3 d S T P . .
K1 K 0.5000 0.5000 0.78036(14) 0.0297(7) Uani 0.623(13) 4 d S T P . .
OW1 O 0.5000 0.5000 0.78036(14) 0.0297(7) Uani 0.377(13) 4 d S T P . .
F1 F 0.5000 0.70584(15) 0.64508(14) 0.0257(6) Uani 1 2 d S T P . .
O1 O 0.40757(13) 0.66391(13) 0.77792(13) 0.0314(6) Uani 1 1 d . . . . .
O21 O 0.41037(16) 0.58963(16) 0.91037(16) 0.0408(12) Uani 0.851(4) 3 d S T P . .
O22 O 0.2728(9) 0.7272(9) 0.7728(9) 0.0408(12) Uani 0.149(4) 3 d S T P . .
O3 O 0.3810(3) 0.5000 0.5000 0.0474(14) Uani 1 4 d S T P . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Mn1 F1 1.818(2) 61_666 ?
Mn1 F1 1.818(2) . ?
Mn1 O1 2.066(2) . ?
Mn1 O1 2.066(2) 61_666 ?
Mn1 O1 2.066(2) 51_655 ?
Mn1 O1 2.066(2) 15_566 ?
Mn1 Na1 3.4924(9) . ?
Mn1 Na1 3.4924(9) 61_666 ?
Mn1 Na1 3.4924(9) 15_566 ?
Mn1 Na1 3.4924(9) 51_655 ?
Mn1 K1 4.0213(6) 61_666 ?
Mn1 K1 4.0213(6) 69_666 ?
Mn2 O3 1.901(5) . ?
Mn2 O3 1.901(5) 57_666 ?
Mn2 O3 1.901(5) 9 ?
Mn2 O3 1.901(5) 53_666 ?
Mn2 O3 1.901(5) 5 ?
Mn2 O3 1.901(5) 49_666 ?
Mn2 Na1 3.355(2) 3_566 ?
Mn2 Na1 3.355(2) 51_655 ?
Mn2 Na1 3.355(2) 49_666 ?
Mn2 Na1 3.355(2) 52_565 ?
Mn2 Na1 3.355(2) 4_656 ?
Mn2 Na1 3.355(2) 50_556 ?
P11 P12 0.713(13) . ?
P11 O1 1.508(2) 24_665 ?
P11 O1 1.508(2) 31_466 ?
P11 O1 1.508(2) . ?
P11 O21 1.580(5) . ?
P11 O22 2.22(2) . ?
P11 K1 3.5123(15) 69_666 ?
P11 K1 3.5123(15) . ?
P11 K1 3.5123(15) 29_455 ?
P12 O1 1.510(4) 24_665 ?
P12 O1 1.510(4) 31_466 ?
P12 O1 1.510(4) . ?
P12 O22 1.51(3) . ?
Na1 F1 2.3913(14) . ?
Na1 F1 2.3913(14) 58_655 ?
Na1 F1 2.3913(14) 6_665 ?
Na1 O1 2.632(3) . ?
Na1 O1 2.632(3) 6_665 ?
Na1 O1 2.632(3) 11_656 ?
Na1 O3 2.7400(19) . ?
Na1 O3 2.7400(19) 57_666 ?
Na1 O3 2.7400(19) 53_666 ?
Na1 Mn1 3.4924(9) 46_466 ?
K1 O3 2.576(5) 57_666 ?
K1 F1 2.604(3) 6_665 ?
K1 F1 2.604(3) 5 ?
K1 O21 2.8994(18) 51_655 ?
K1 O21 2.8994(18) 2_665 ?
K1 O21 2.8994(18) 52_565 ?
K1 O21 2.8994(18) . ?
K1 O1 3.005(2) . ?
K1 O1 3.005(2) 52_565 ?
K1 O1 3.005(2) 51_655 ?
K1 O1 3.005(2) 2_665 ?
K1 P11 3.5123(15) 51_655 ?
F1 Na1 2.3913(14) 51_655 ?
F1 K1 2.604(3) 9 ?
O21 K1 2.8994(18) 69_666 ?
O21 K1 2.8994(18) 29_455 ?
O22 O22 1.03(4) 28_556 ?
O22 O22 1.03(4) 15_566 ?
O22 O22 1.03(4) 38_565 ?
O3 K1 2.576(5) 53_666 ?
O3 Na1 2.7400(19) 3_566 ?
O3 Na1 2.7400(19) 52_565 ?
O3 Na1 2.7400(19) 50_556 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
F1 Mn1 F1 180.0 61_666 . ?
F1 Mn1 O1 93.40(8) 61_666 . ?
F1 Mn1 O1 86.60(8) . . ?
F1 Mn1 O1 86.60(8) 61_666 61_666 ?
F1 Mn1 O1 93.40(8) . 61_666 ?
O1 Mn1 O1 180.0 . 61_666 ?
F1 Mn1 O1 93.40(8) 61_666 51_655 ?
F1 Mn1 O1 86.60(8) . 51_655 ?
O1 Mn1 O1 91.21(12) . 51_655 ?
O1 Mn1 O1 88.79(12) 61_666 51_655 ?
F1 Mn1 O1 86.60(8) 61_666 15_566 ?
F1 Mn1 O1 93.40(8) . 15_566 ?
O1 Mn1 O1 88.79(12) . 15_566 ?
O1 Mn1 O1 91.21(12) 61_666 15_566 ?
O1 Mn1 O1 180.0 51_655 15_566 ?
F1 Mn1 Na1 140.40(5) 61_666 . ?
F1 Mn1 Na1 39.60(5) . . ?
O1 Mn1 Na1 48.63(6) . . ?
O1 Mn1 Na1 131.37(6) 61_666 . ?
O1 Mn1 Na1 97.57(6) 51_655 . ?
O1 Mn1 Na1 82.43(6) 15_566 . ?
F1 Mn1 Na1 39.60(5) 61_666 61_666 ?
F1 Mn1 Na1 140.40(5) . 61_666 ?
O1 Mn1 Na1 131.37(6) . 61_666 ?
O1 Mn1 Na1 48.63(6) 61_666 61_666 ?
O1 Mn1 Na1 82.43(6) 51_655 61_666 ?
O1 Mn1 Na1 97.57(6) 15_566 61_666 ?
Na1 Mn1 Na1 180.0 . 61_666 ?
F1 Mn1 Na1 39.60(5) 61_666 15_566 ?
F1 Mn1 Na1 140.40(5) . 15_566 ?
O1 Mn1 Na1 82.43(6) . 15_566 ?
O1 Mn1 Na1 97.57(6) 61_666 15_566 ?
O1 Mn1 Na1 131.37(6) 51_655 15_566 ?
O1 Mn1 Na1 48.63(6) 15_566 15_566 ?
Na1 Mn1 Na1 112.62(7) . 15_566 ?
Na1 Mn1 Na1 67.38(7) 61_666 15_566 ?
F1 Mn1 Na1 140.40(5) 61_666 51_655 ?
F1 Mn1 Na1 39.60(5) . 51_655 ?
O1 Mn1 Na1 97.57(6) . 51_655 ?
O1 Mn1 Na1 82.43(6) 61_666 51_655 ?
O1 Mn1 Na1 48.63(6) 51_655 51_655 ?
O1 Mn1 Na1 131.37(6) 15_566 51_655 ?
Na1 Mn1 Na1 67.38(7) . 51_655 ?
Na1 Mn1 Na1 112.62(7) 61_666 51_655 ?
Na1 Mn1 Na1 180.0 15_566 51_655 ?
F1 Mn1 K1 74.10(8) 61_666 61_666 ?
F1 Mn1 K1 105.90(8) . 61_666 ?
O1 Mn1 K1 133.37(6) . 61_666 ?
O1 Mn1 K1 46.64(6) 61_666 61_666 ?
O1 Mn1 K1 133.36(6) 51_655 61_666 ?
O1 Mn1 K1 46.64(6) 15_566 61_666 ?
Na1 Mn1 K1 120.87(3) . 61_666 ?
Na1 Mn1 K1 59.13(3) 61_666 61_666 ?
Na1 Mn1 K1 59.13(3) 15_566 61_666 ?
Na1 Mn1 K1 120.87(3) 51_655 61_666 ?
F1 Mn1 K1 29.75(8) 61_666 69_666 ?
F1 Mn1 K1 150.25(8) . 69_666 ?
O1 Mn1 K1 72.88(6) . 69_666 ?
O1 Mn1 K1 107.12(6) 61_666 69_666 ?
O1 Mn1 K1 72.88(6) 51_655 69_666 ?
O1 Mn1 K1 107.12(6) 15_566 69_666 ?
Na1 Mn1 K1 120.87(3) . 69_666 ?
Na1 Mn1 K1 59.13(3) 61_666 69_666 ?
Na1 Mn1 K1 59.13(3) 15_566 69_666 ?
Na1 Mn1 K1 120.87(3) 51_655 69_666 ?
K1 Mn1 K1 103.85(6) 61_666 69_666 ?
O3 Mn2 O3 90.000(1) . 57_666 ?
O3 Mn2 O3 90.0 . 9 ?
O3 Mn2 O3 180.0 57_666 9 ?
O3 Mn2 O3 90.0 . 53_666 ?
O3 Mn2 O3 90.0 57_666 53_666 ?
O3 Mn2 O3 90.0 9 53_666 ?
O3 Mn2 O3 90.000(1) . 5 ?
O3 Mn2 O3 90.0 57_666 5 ?
O3 Mn2 O3 90.0 9 5 ?
O3 Mn2 O3 180.0 53_666 5 ?
O3 Mn2 O3 180.0 . 49_666 ?
O3 Mn2 O3 90.000(1) 57_666 49_666 ?
O3 Mn2 O3 90.0 9 49_666 ?
O3 Mn2 O3 90.000(1) 53_666 49_666 ?
O3 Mn2 O3 90.0 5 49_666 ?
O3 Mn2 Na1 54.7 . 3_566 ?
O3 Mn2 Na1 125.264(1) 57_666 3_566 ?
O3 Mn2 Na1 54.7 9 3_566 ?
O3 Mn2 Na1 125.3 53_666 3_566 ?
O3 Mn2 Na1 54.7 5 3_566 ?
O3 Mn2 Na1 125.3 49_666 3_566 ?
O3 Mn2 Na1 125.3 . 51_655 ?
O3 Mn2 Na1 54.736(1) 57_666 51_655 ?
O3 Mn2 Na1 125.3 9 51_655 ?
O3 Mn2 Na1 54.7 53_666 51_655 ?
O3 Mn2 Na1 125.3 5 51_655 ?
O3 Mn2 Na1 54.7 49_666 51_655 ?
Na1 Mn2 Na1 180.00(4) 3_566 51_655 ?
O3 Mn2 Na1 125.3 . 49_666 ?
O3 Mn2 Na1 125.3 57_666 49_666 ?
O3 Mn2 Na1 54.7 9 49_666 ?
O3 Mn2 Na1 125.3 53_666 49_666 ?
O3 Mn2 Na1 54.7 5 49_666 ?
O3 Mn2 Na1 54.7 49_666 49_666 ?
Na1 Mn2 Na1 70.5 3_566 49_666 ?
Na1 Mn2 Na1 109.5 51_655 49_666 ?
O3 Mn2 Na1 54.7 . 52_565 ?
O3 Mn2 Na1 54.736(1) 57_666 52_565 ?
O3 Mn2 Na1 125.264(1) 9 52_565 ?
O3 Mn2 Na1 125.3 53_666 52_565 ?
O3 Mn2 Na1 54.7 5 52_565 ?
O3 Mn2 Na1 125.3 49_666 52_565 ?
Na1 Mn2 Na1 70.5 3_566 52_565 ?
Na1 Mn2 Na1 109.5 51_655 52_565 ?
Na1 Mn2 Na1 109.5 49_666 52_565 ?
O3 Mn2 Na1 125.3 . 4_656 ?
O3 Mn2 Na1 125.264(1) 57_666 4_656 ?
O3 Mn2 Na1 54.7 9 4_656 ?
O3 Mn2 Na1 54.7 53_666 4_656 ?
O3 Mn2 Na1 125.3 5 4_656 ?
O3 Mn2 Na1 54.7 49_666 4_656 ?
Na1 Mn2 Na1 109.5 3_566 4_656 ?
Na1 Mn2 Na1 70.5 51_655 4_656 ?
Na1 Mn2 Na1 70.5 49_666 4_656 ?
Na1 Mn2 Na1 180.00(4) 52_565 4_656 ?
O3 Mn2 Na1 54.7 . 50_556 ?
O3 Mn2 Na1 125.3 57_666 50_556 ?
O3 Mn2 Na1 54.7 9 50_556 ?
O3 Mn2 Na1 54.7 53_666 50_556 ?
O3 Mn2 Na1 125.3 5 50_556 ?
O3 Mn2 Na1 125.3 49_666 50_556 ?
Na1 Mn2 Na1 70.5 3_566 50_556 ?
Na1 Mn2 Na1 109.471(1) 51_655 50_556 ?
Na1 Mn2 Na1 109.5 49_666 50_556 ?
Na1 Mn2 Na1 109.5 52_565 50_556 ?
Na1 Mn2 Na1 70.5 4_656 50_556 ?
P12 P11 O1 76.50(12) . 24_665 ?
P12 P11 O1 76.50(12) . 31_466 ?
O1 P11 O1 114.72(9) 24_665 31_466 ?
P12 P11 O1 76.50(12) . . ?
O1 P11 O1 114.72(9) 24_665 . ?
O1 P11 O1 114.72(9) 31_466 . ?
P12 P11 O21 180.0(4) . . ?
O1 P11 O21 103.50(12) 24_665 . ?
O1 P11 O21 103.50(12) 31_466 . ?
O1 P11 O21 103.50(12) . . ?
P12 P11 O22 0.0(5) . . ?
O1 P11 O22 76.50(12) 24_665 . ?
O1 P11 O22 76.50(12) 31_466 . ?
O1 P11 O22 76.50(12) . . ?
O21 P11 O22 180.0(4) . . ?
P12 P11 K1 125.38(5) . 69_666 ?
O1 P11 K1 58.21(10) 24_665 69_666 ?
O1 P11 K1 147.56(11) 31_466 69_666 ?
O1 P11 K1 95.07(9) . 69_666 ?
O21 P11 K1 54.62(5) . 69_666 ?
O22 P11 K1 125.38(5) . 69_666 ?
P12 P11 K1 125.38(5) . . ?
O1 P11 K1 147.56(12) 24_665 . ?
O1 P11 K1 95.07(9) 31_466 . ?
O1 P11 K1 58.21(10) . . ?
O21 P11 K1 54.62(5) . . ?
O22 P11 K1 125.38(5) . . ?
K1 P11 K1 89.83(6) 69_666 . ?
P12 P11 K1 125.38(5) . 29_455 ?
O1 P11 K1 95.07(9) 24_665 29_455 ?
O1 P11 K1 58.21(10) 31_466 29_455 ?
O1 P11 K1 147.56(11) . 29_455 ?
O21 P11 K1 54.62(5) . 29_455 ?
O22 P11 K1 125.38(5) . 29_455 ?
K1 P11 K1 89.83(6) 69_666 29_455 ?
K1 P11 K1 89.83(6) . 29_455 ?
P11 P12 O1 76.2(5) . 24_665 ?
P11 P12 O1 76.2(5) . 31_466 ?
O1 P12 O1 114.5(4) 24_665 31_466 ?
P11 P12 O1 76.2(5) . . ?
O1 P12 O1 114.5(4) 24_665 . ?
O1 P12 O1 114.5(4) 31_466 . ?
P11 P12 O22 180(2) . . ?
O1 P12 O22 103.8(5) 24_665 . ?
O1 P12 O22 103.8(5) 31_466 . ?
O1 P12 O22 103.8(5) . . ?
F1 Na1 F1 119.749(12) . 58_655 ?
F1 Na1 F1 119.749(12) . 6_665 ?
F1 Na1 F1 119.749(12) 58_655 6_665 ?
F1 Na1 O1 63.99(7) . . ?
F1 Na1 O1 145.85(11) 58_655 . ?
F1 Na1 O1 72.60(7) 6_665 . ?
F1 Na1 O1 145.85(11) . 6_665 ?
F1 Na1 O1 72.60(7) 58_655 6_665 ?
F1 Na1 O1 63.99(7) 6_665 6_665 ?
O1 Na1 O1 88.07(9) . 6_665 ?
F1 Na1 O1 72.60(7) . 11_656 ?
F1 Na1 O1 63.99(7) 58_655 11_656 ?
F1 Na1 O1 145.85(11) 6_665 11_656 ?
O1 Na1 O1 88.07(9) . 11_656 ?
O1 Na1 O1 88.07(9) 6_665 11_656 ?
F1 Na1 O3 120.03(12) . . ?
F1 Na1 O3 63.05(9) 58_655 . ?
F1 Na1 O3 80.11(6) 6_665 . ?
O1 Na1 O3 148.43(7) . . ?
O1 Na1 O3 94.09(10) 6_665 . ?
O1 Na1 O3 123.45(6) 11_656 . ?
F1 Na1 O3 80.11(6) . 57_666 ?
F1 Na1 O3 120.03(12) 58_655 57_666 ?
F1 Na1 O3 63.05(9) 6_665 57_666 ?
O1 Na1 O3 94.09(10) . 57_666 ?
O1 Na1 O3 123.45(6) 6_665 57_666 ?
O1 Na1 O3 148.44(7) 11_656 57_666 ?
O3 Na1 O3 58.76(16) . 57_666 ?
F1 Na1 O3 63.05(9) . 53_666 ?
F1 Na1 O3 80.11(6) 58_655 53_666 ?
F1 Na1 O3 120.03(12) 6_665 53_666 ?
O1 Na1 O3 123.45(6) . 53_666 ?
O1 Na1 O3 148.44(7) 6_665 53_666 ?
O1 Na1 O3 94.09(10) 11_656 53_666 ?
O3 Na1 O3 58.76(16) . 53_666 ?
O3 Na1 O3 58.76(16) 57_666 53_666 ?
F1 Na1 Mn2 87.12(7) . . ?
F1 Na1 Mn2 87.12(7) 58_655 . ?
F1 Na1 Mn2 87.12(7) 6_665 . ?
O1 Na1 Mn2 126.62(6) . . ?
O1 Na1 Mn2 126.62(6) 6_665 . ?
O1 Na1 Mn2 126.62(6) 11_656 . ?
O3 Na1 Mn2 34.50(10) . . ?
O3 Na1 Mn2 34.50(10) 57_666 . ?
O3 Na1 Mn2 34.50(10) 53_666 . ?
F1 Na1 Mn1 28.98(5) . . ?
F1 Na1 Mn1 134.14(7) 58_655 . ?
F1 Na1 Mn1 103.45(6) 6_665 . ?
O1 Na1 Mn1 36.08(4) . . ?
O1 Na1 Mn1 118.56(8) 6_665 . ?
O1 Na1 Mn1 71.79(5) 11_656 . ?
O3 Na1 Mn1 145.55(11) . . ?
O3 Na1 Mn1 91.81(6) 57_666 . ?
O3 Na1 Mn1 91.81(6) 53_666 . ?
Mn2 Na1 Mn1 111.04(3) . . ?
F1 Na1 Mn1 103.45(6) . 46_466 ?
F1 Na1 Mn1 28.98(5) 58_655 46_466 ?
F1 Na1 Mn1 134.14(7) 6_665 46_466 ?
O1 Na1 Mn1 118.56(8) . 46_466 ?
O1 Na1 Mn1 71.79(5) 6_665 46_466 ?
O1 Na1 Mn1 36.08(4) 11_656 46_466 ?
O3 Na1 Mn1 91.81(6) . 46_466 ?
O3 Na1 Mn1 145.55(11) 57_666 46_466 ?
O3 Na1 Mn1 91.81(6) 53_666 46_466 ?
Mn2 Na1 Mn1 111.04(3) . 46_466 ?
Mn1 Na1 Mn1 107.85(4) . 46_466 ?
O3 K1 F1 62.81(7) 57_666 6_665 ?
O3 K1 F1 62.81(7) 57_666 5 ?
F1 K1 F1 125.63(13) 6_665 5 ?
O3 K1 O21 135.73(9) 57_666 51_655 ?
F1 K1 O21 140.02(5) 6_665 51_655 ?
F1 K1 O21 83.58(8) 5 51_655 ?
O3 K1 O21 135.73(9) 57_666 2_665 ?
F1 K1 O21 140.02(5) 6_665 2_665 ?
F1 K1 O21 83.58(8) 5 2_665 ?
O21 K1 O21 59.15(11) 51_655 2_665 ?
O3 K1 O21 135.73(9) 57_666 52_565 ?
F1 K1 O21 83.58(8) 6_665 52_565 ?
F1 K1 O21 140.02(5) 5 52_565 ?
O21 K1 O21 88.54(19) 51_655 52_565 ?
O21 K1 O21 59.15(11) 2_665 52_565 ?
O3 K1 O21 135.73(9) 57_666 . ?
F1 K1 O21 83.57(8) 6_665 . ?
F1 K1 O21 140.02(5) 5 . ?
O21 K1 O21 59.15(11) 51_655 . ?
O21 K1 O21 88.54(19) 2_665 . ?
O21 K1 O21 59.15(11) 52_565 . ?
O3 K1 O1 89.26(6) 57_666 . ?
F1 K1 O1 63.71(4) 6_665 . ?
F1 K1 O1 115.53(5) 5 . ?
O21 K1 O1 79.74(5) 51_655 . ?
O21 K1 O1 132.97(12) 2_665 . ?
O21 K1 O1 101.35(5) 52_565 . ?
O21 K1 O1 48.47(9) . . ?
O3 K1 O1 89.26(6) 57_666 52_565 ?
F1 K1 O1 63.71(4) 6_665 52_565 ?
F1 K1 O1 115.53(5) 5 52_565 ?
O21 K1 O1 132.97(12) 51_655 52_565 ?
O21 K1 O1 79.74(5) 2_665 52_565 ?
O21 K1 O1 48.47(9) 52_565 52_565 ?
O21 K1 O1 101.35(5) . 52_565 ?
O1 K1 O1 121.14(8) . 52_565 ?
O3 K1 O1 89.26(6) 57_666 51_655 ?
F1 K1 O1 115.53(5) 6_665 51_655 ?
F1 K1 O1 63.71(4) 5 51_655 ?
O21 K1 O1 48.47(9) 51_655 51_655 ?
O21 K1 O1 101.35(5) 2_665 51_655 ?
O21 K1 O1 132.97(12) 52_565 51_655 ?
O21 K1 O1 79.74(5) . 51_655 ?
O1 K1 O1 58.84(8) . 51_655 ?
O1 K1 O1 178.51(11) 52_565 51_655 ?
O3 K1 O1 89.26(6) 57_666 2_665 ?
F1 K1 O1 115.53(5) 6_665 2_665 ?
F1 K1 O1 63.71(4) 5 2_665 ?
O21 K1 O1 101.35(5) 51_655 2_665 ?
O21 K1 O1 48.47(9) 2_665 2_665 ?
O21 K1 O1 79.74(5) 52_565 2_665 ?
O21 K1 O1 132.97(12) . 2_665 ?
O1 K1 O1 178.51(11) . 2_665 ?
O1 K1 O1 58.84(8) 52_565 2_665 ?
O1 K1 O1 121.14(8) 51_655 2_665 ?
O3 K1 P11 109.35(5) 57_666 51_655 ?
F1 K1 P11 138.147(16) 6_665 51_655 ?
F1 K1 P11 63.77(4) 5 51_655 ?
O21 K1 P11 26.38(9) 51_655 51_655 ?
O21 K1 P11 76.27(4) 2_665 51_655 ?
O21 K1 P11 114.92(11) 52_565 51_655 ?
O21 K1 P11 76.27(4) . 51_655 ?
O1 K1 P11 75.58(4) . 51_655 ?
O1 K1 P11 155.93(8) 52_565 51_655 ?
O1 K1 P11 25.25(4) 51_655 51_655 ?
O1 K1 P11 104.93(4) 2_665 51_655 ?
Mn1 F1 Na1 111.42(8) . 51_655 ?
Mn1 F1 Na1 111.42(8) . . ?
Na1 F1 Na1 108.22(13) 51_655 . ?
Mn1 F1 K1 129.99(12) . 9 ?
Na1 F1 K1 96.70(7) 51_655 9 ?
Na1 F1 K1 96.70(7) . 9 ?
P11 O1 P12 27.3(5) . . ?
P11 O1 Mn1 134.74(13) . . ?
P12 O1 Mn1 131.1(2) . . ?
P11 O1 Na1 127.60(12) . . ?
P12 O1 Na1 111.9(4) . . ?
Mn1 O1 Na1 95.29(8) . . ?
P11 O1 K1 96.54(12) . . ?
P12 O1 K1 119.3(4) . . ?
Mn1 O1 K1 103.38(8) . . ?
Na1 O1 K1 82.73(8) . . ?
P11 O21 K1 99.01(9) . . ?
P11 O21 K1 99.01(9) . 69_666 ?
K1 O21 K1 117.60(5) . 69_666 ?
P11 O21 K1 99.01(9) . 29_455 ?
K1 O21 K1 117.60(5) . 29_455 ?
K1 O21 K1 117.60(5) 69_666 29_455 ?
O22 O22 O22 59.997(1) 28_556 15_566 ?
O22 O22 O22 59.997(3) 28_556 38_565 ?
O22 O22 O22 59.997(3) 15_566 38_565 ?
O22 O22 P12 144.737(11) 28_556 . ?
O22 O22 P12 144.737(12) 15_566 . ?
O22 O22 P12 144.737(7) 38_565 . ?
O22 O22 P11 144.737(9) 28_556 . ?
O22 O22 P11 144.737(9) 15_566 . ?
O22 O22 P11 144.737(5) 38_565 . ?
P12 O22 P11 0.0(5) . . ?
Mn2 O3 K1 180.0 . 53_666 ?
Mn2 O3 Na1 90.76(10) . 3_566 ?
K1 O3 Na1 89.24(10) 53_666 3_566 ?
Mn2 O3 Na1 90.76(10) . 52_565 ?
K1 O3 Na1 89.24(10) 53_666 52_565 ?
Na1 O3 Na1 89.990(3) 3_566 52_565 ?
Mn2 O3 Na1 90.76(10) . 50_556 ?
K1 O3 Na1 89.24(10) 53_666 50_556 ?
Na1 O3 Na1 89.990(3) 3_566 50_556 ?
Na1 O3 Na1 178.48(19) 52_565 50_556 ?
Mn2 O3 Na1 90.76(10) . . ?
K1 O3 Na1 89.24(10) 53_666 . ?
Na1 O3 Na1 178.48(19) 3_566 . ?
Na1 O3 Na1 89.990(3) 52_565 . ?
Na1 O3 Na1 89.990(3) 50_556 . ?
 
_refine_diff_density_max    0.780
_refine_diff_density_min   -0.742
_refine_diff_density_rms    0.119

_shelxl_version_number 2013-2



